Structural insights into the thermal decomposition sequence of barium tetrahydrogenorthotellurate(VI), Ba[H4TeO6]
Matthias Weila; Berthold Stogera; Christian Gierl-Mayerb; Eugen Libowitzkyc; Journal of Solid State Chemistry 241 (2016) 187–197; doi:10.1016/j.jssc.2016.06.010

data_1543545
_publ_section_title
;
 Structural insights into the thermal decomposition sequence of barium
 tetrahydrogenorthotellurate(VI), Ba[H4TeO6]
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              187
_journal_page_last               197
_journal_paper_doi               10.1016/j.jssc.2016.06.010
_journal_volume                  241
_journal_year                    2016
_chemical_formula_sum            'Ba H4 O6 Te'
_chemical_formula_weight         364.97
_chemical_name_systematic
; 
Barium tetrahydrogenhexaoxotellurate(VI) 
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   .
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 106.443(2)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.8271(7)
_cell_length_b                   7.9998(7)
_cell_length_c                   8.4624(8)
_cell_measurement_reflns_used    3270
_cell_measurement_temperature    295(2)
_cell_measurement_theta_max      30.975
_cell_measurement_theta_min      3.132
_cell_volume                     508.20(8)
_computing_cell_refinement       SAINT
_computing_data_collection       SMART
_computing_data_reduction        SAINT
_computing_molecular_graphics    ATOMS
_computing_publication_material  SHELX-L97
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      295(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.986
_diffrn_measurement_device_type  'SMART Apex CCD'
_diffrn_measurement_method       \w
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0363
_diffrn_reflns_av_unetI/netI     0.0356
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.986
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            5876
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.986
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         30.985
_diffrn_reflns_theta_min         3.132
_exptl_absorpt_coefficient_mu    13.386
_exptl_absorpt_correction_T_max  0.7946
_exptl_absorpt_correction_T_min  0.2965
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS (Bruker, 2010)
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    4.770
_exptl_crystal_description       plate
_exptl_crystal_F_000             640
_exptl_crystal_size_max          0.120
_exptl_crystal_size_mid          0.120
_exptl_crystal_size_min          0.018
_refine_diff_density_max         1.621
_refine_diff_density_min         -1.136
_refine_diff_density_rms         0.276
_refine_ls_extinction_coef       0.0011(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014)'
_refine_ls_goodness_of_fit_ref   1.094
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     75
_refine_ls_number_reflns         1603
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.094
_refine_ls_R_factor_all          0.0273
_refine_ls_R_factor_gt           0.0244
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0313P)^2^+0.8718P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0643
_refine_ls_wR_factor_ref         0.0659
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                1472
_reflns_number_total             1603
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            BaH4TeO6.cif
_cod_data_source_block           BaH4TeO6
_cod_depositor_comments
;
The following automatic conversions were performed:

'_journal_paper_doi' value 'doi:10.1016/j.jssc.2016.06.010' was
changed to '10.1016/j.jssc.2016.06.010'.

Automatic conversion script
Id: cif_fix_values 6433 2018-09-21 13:16:33Z andrius 
;
_cod_database_code               1543545
_shelx_estimated_absorpt_t_min   0.296
_shelx_estimated_absorpt_t_max   0.795